SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez nos Conditions d’utilisation et notre Politique de confidentialité.

SlideShare utilise les cookies pour améliorer les fonctionnalités et les performances, et également pour vous montrer des publicités pertinentes. Si vous continuez à naviguer sur ce site, vous acceptez l’utilisation de cookies. Consultez notre Politique de confidentialité et nos Conditions d’utilisation pour en savoir plus.

Ce diaporama a bien été signalé.

Vous avez aimé cette présentation ? Partagez !

4 564 vues

Publié le

Based on a paper by Sunil.

Publié dans :
Ingénierie

Aucun téléchargement

Nombre de vues

4 564

Sur SlideShare

0

Issues des intégrations

0

Intégrations

0

Partages

0

Téléchargements

255

Commentaires

5

J’aime

9

Aucune remarque pour cette diapositive

- 1. RECYCLED AGGREGATE CONCRETE The International Reviewer Volume 1 | Issue 2 | July - December 2014 | pp. 30-33 | ISSN 2395-1575 Sunil, A. U. Ravishankar, Suresha S. N., S. M. Naik Presentation by: Ahmad Shah Kakar, Tsegaye Arega, Shamsuddin Masoud Indian Institute of Technology-Delhi, Hauz Khas, New Delhi, Delhi 110016 2017
- 2. CONTENTS INTRODUCTION LITERATURE SURVEY EXPERIMENTAL METHODOLOGY: PROCESSING OF RAC RESULTS AND DISCUSSION i) Properties of RAC ii) Mix Proportions iii) Slump Test IV) Compression Test V) Modulus of Elasticity Test CONCLUSION REFERENCES
- 3. Introduction Recycled aggregate are comprised of crushed, graded inorganic particles processed from the materials that have been used in the construction and demolition debris. These materials are generally from buildings, roads, bridges, and sometimes even from catastrophes, such as wars and earthquakes. Recycled aggregate is generally produced by two stages crushing of demolished concrete, screening and removal of contaminants such as reinforcement, plastic etc. Concrete made with such aggregates is called as Recycled aggregate Concrete (RAC). Demolition of old and deteriorated buildings and traffic infrastructure, and their substitution with new ones, is a frequent phenomenon today in a large part of the world.
- 4. Introduction Recent research of Freedonia group has found: Global demand of aggregates for construction 46 billion metric tons in 2011 51 billion metric tons in 2019
- 5. In addition… Construction and demolition wastes are generated annually in world 14.5 Million Tons (India) 13 Million Tons (France) 10-15 Million Tons (Japan) 20 Million Tons ( Hong Kong) Investigation results of Environmental resources ltd(1979) for EEC (European Economic Community) member countries found 55 Million Tons - by 1980 302 Million Tons – by 2020
- 6. LITERATURE SURVEY Limbachiya and Leelawat (2000) found that recycled aggregate concrete had 7 to 9% lower relative density and 2 times higher water absorption than natural aggregate. According to Bodin and Zaharieva, precautions must also be taken of pathological reactions such as alkali – aggregate reaction and sulphate reaction in the industrially produced recycled aggregate.
- 7. EXPERIMENTAL METHODOLOGY: PROCESSING OF RAC In this project, the recycled concrete aggregates are obtained from the big concrete blocks. These blocks are first crushed by using Hammer to a size of 40mm or less then it is crushed by using Crusher. Due to this the recycled aggregates of size 10mm to 20mm are obtained. These recycled aggregates are wet they are dried by keeping in oven for 24 days. The different tests are carried out on finally obtained recycled aggregates and Mix design of concrete of grade M20 by using IS 1260:2009 and 456:2000.
- 8. RESULTS AND DISCUSSION i) Properties of RAC Sum of Cumulative Percentage Retained = 533.8 Fineness Modulus = 533.8/100 = 5.338 IS Sieve Weight Retained (kg) Cumulative Weight Retained (kg) Cumulative Percentage Weight Retained (%) Cumulative Percentage Passing (%) 40mm 0 0 0 100 20mm 0.1750 0.170 3.4 96.6 10mm 2.475 2.645 52.9 47.1 4.75mm 1.806 4.451 89.02 10.98 2.36mm 0.23 4.681 93.62 6.38 1.18mm 0.15 4.831 96.62 3.38 600micron 0.10 4.931 98.62 1.38 150micron 0.05 4.981 99.62 0.38 Properties Recycled Aggregate Concrete Specific gravity 2.57 Water absorption 1.21% Aggregate Impact Value 30.69% Aggregate Crushing Value 29.86% Table 1: Particule Size Distribution. Table 2: Properties of RAC.
- 9. ii) Mix Proportions The compressive strength increased with a decrease in w/c ratio and is directly proportional to strength of blended aggregate. However, when used at higher level of replacement, the high water absorption ability of recycled aggregate resulted in the higher total water demand. We Know that, Target Strength for M20 Mix proportion is 20 + (1.65x4) as equal to 26.6MPa and the Ratio of Cement : Sand : aggregate was arrived at as 1:2.65:3.92. The results are tabulated under Table Cement 300kg/m3 Water 148.8 kg/m3 Fine aggregate 796kg Coarse aggregate 1173.462kg Water – Cement ratio 0.50 Fine aggregate to Cement ratio 2.65 Coarse aggregate to Cement ratio 3.92 Slump 50mm Table 3: Mix Proportion.
- 10. iii) Slump Test Slump test was used to determine the workability of fresh concrete. The slump less than 25mm indicates a very stiff concrete and a slump that more than 125mm indicates a running concrete. The results indicated 48mm for 100% recycled aggregate and 55 mm for 75% recycled aggregate. The results are tabulated under Table 4. Percentage of Recycled Aggregate (%) Slump (mm) 100% recycled aggregate 48 75% recycled aggregate 55 Table 4: Variation of Slump with Percentage of RAC.
- 11. IV) Compression Test A Concrete mix having cement, fine aggregate and coarse aggregate in the ratio of 1:2.65:3.92 was prepared. The components were mixed using machine in adding water cement ratio of 0.50 during the process. The concrete mix was filled in 9 cube moulds kept for 24 hours. After 24 hours, the specimens were demoulded and kept immersed in water for 7, 14 and 21 days after which they were removed for testing. The results are tabulated under Table 5. Percentage of Recycled Aggregate Concrete Compressive Strength for 7days (MPa) Compressive Strength for 14days (MPa) Compressive Strength for 21days (MPa) 100% 21.24 23.62 24.88 75% 23.70 24.98 25.99 Table 5: Variation of Compressive Strength.
- 12. Compression Test
- 13. V) Modulus of Elasticity Test Moulded test specimens (cylinders) were of the size 150x300mm. 3 such specimens were prepared using same concrete mix design as compressive strength and tested after 21 days of curing. The results are presented under Chart 1.
- 14. VI) Splitting Tensile Strength Test of Concrete. Moulded test specimens (cylinders) are of the size 150x300mm. 3 such specimens were prepared using same concrete mix design and tested after 21days of curing. The results are tabulated under Table 6. Specimens Weight of Cylinder (kg) Ultimate Load P (KN) Split Tensile Strength (MPa) 2P/ (ΠDL) 1 12.56 190 2.63 2 12.46 180 2.54 3 12.60 195 2.75 Table 6: Variation of Splitting Tensile Strength with Ultimate Load.
- 15. Splitting Tensile Strength Test of Concrete.
- 16. CONCLUSION Using Recycled fine aggregates in concrete can prove to be better however in less quantity and can be recommended for lower grade applications like lower layers of roads such Sub base course and base course. By using Recycled aggregates in construction it will maximize the economic and environmental benefits. Compressive Strength of Concrete will decreases with increase in Percentage of Recycled Aggregates for 7, 14, 21 days. The Modulus of Elasticity of Concrete is an important property in Mix Design. The modulus of elasticity of concrete also affects its strength. Splitting Tensile Strength Test is simple and gives uniform results. The Average Tensile Strength is 2.65MPa for 21 days test specimen. Average Compressive Strength for 100% of Recycled aggregate at 21days specimen is 24.98MPa. Average Compressive Strength for 75% of Recycled aggregate at 21days specimen is 25.99MPa.
- 17. REFERENCES [1] Limbachiya M.C., Leelawat T. and Dhir R.K.; Use of recycled concrete aggregate in high-strength concrete, Materials and Structures, Vol. 33, pp. 574-580, 2000. [2] Buyle-Bodin F. and Hadijieva-Zaharieva R.; Influence of industrially produced recycled aggregates on flow properties of concrete, Materials and Structures, Vol. 35, pp. 504-509, 2002.

Aucun clipboard public n’a été trouvé avec cette diapositive

Il semblerait que vous ayez déjà ajouté cette diapositive à .

Créer un clipboard

Identifiez-vous pour voir les commentaires